#------------------------------------------------------------------------------
#$Date: 2021-03-29 12:15:25 +0300 (Mon, 29 Mar 2021) $
#$Revision: 263414 $
#$URL: file:///home/coder/svn-repositories/cod/cif/1/56/13/1561331.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/
#
# All data on this site have been placed in the public domain by the
# contributors.
#
data_1561331
loop_
_publ_author_name
'Li, Shujun'
'Peng, Qingpo'
'Chen, Xuenian'
'Wang, Ruoya'
'Zhai, Jianxin'
'Hu, Weihua'
'Ma, Fengji'
'Zhang, Jie'
'Liu, Shuxia'
_publ_section_title
;
 A Ta/W mixed addenda heteropolyacid with excellent acid catalytic
 activity and proton-conducting property
;
_journal_name_full               'Journal of Solid State Chemistry'
_journal_page_first              1
_journal_page_last               7
_journal_paper_doi               10.1016/j.jssc.2016.08.003
_journal_volume                  243
_journal_year                    2016
_chemical_formula_sum            'O357 P8 Ta12 W60'
_chemical_formula_weight         19162.16
_space_group_IT_number           114
_space_group_name_Hall           'P -4 2n'
_space_group_name_H-M_alt        'P -4 21 c'
_symmetry_cell_setting           tetragonal
_symmetry_space_group_name_H-M   'P -4 21 c'
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_cell_angle_alpha                90.00
_cell_angle_beta                 90.00
_cell_angle_gamma                90.00
_cell_formula_units_Z            2
_cell_length_a                   24.185(2)
_cell_length_b                   24.185(2)
_cell_length_c                   27.067(3)
_cell_measurement_reflns_used    9953
_cell_measurement_temperature    103(2)
_cell_measurement_theta_max      24.47
_cell_measurement_theta_min      2.38
_cell_volume                     15832(3)
_computing_structure_refinement  'SHELXL-97 (Sheldrick, 2008)'
_computing_structure_solution    'SHELXS-97 (Sheldrick, 2008)'
_diffrn_ambient_temperature      103(2)
_diffrn_measured_fraction_theta_full 0.997
_diffrn_measured_fraction_theta_max 0.997
_diffrn_measurement_device_type  CCD
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_source         'fine-focus sealed tube'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.1714
_diffrn_reflns_av_sigmaI/netI    0.2954
_diffrn_reflns_limit_h_max       20
_diffrn_reflns_limit_h_min       -20
_diffrn_reflns_limit_k_max       29
_diffrn_reflns_limit_k_min       0
_diffrn_reflns_limit_l_max       32
_diffrn_reflns_limit_l_min       -32
_diffrn_reflns_number            28900
_diffrn_reflns_theta_full        25.36
_diffrn_reflns_theta_max         25.36
_diffrn_reflns_theta_min         1.41
_exptl_absorpt_coefficient_mu    25.989
_exptl_absorpt_correction_T_max  0.0782
_exptl_absorpt_correction_T_min  0.0475
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_process_details   sadabs
_exptl_crystal_colour            colorless
_exptl_crystal_density_diffrn    4.020
_exptl_crystal_density_method    'not measured'
_exptl_crystal_description       block
_exptl_crystal_F_000             16584
_exptl_crystal_size_max          0.30
_exptl_crystal_size_mid          0.26
_exptl_crystal_size_min          0.20
_refine_diff_density_max         2.266
_refine_diff_density_min         -2.403
_refine_diff_density_rms         0.354
_refine_ls_abs_structure_details 'Flack H D (1983), Acta Cryst. A39, 876-881'
_refine_ls_abs_structure_Flack   0.00(6)
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   0.889
_refine_ls_matrix_type           full
_refine_ls_number_parameters     1024
_refine_ls_number_reflns         14471
_refine_ls_number_restraints     853
_refine_ls_restrained_S_all      0.870
_refine_ls_R_factor_all          0.1574
_refine_ls_R_factor_gt           0.0841
_refine_ls_shift/su_max          0.008
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'calc w=1/[σ²(Fo²)+(0.0000P)²+0.0000P] where P=(Fo²+2Fc²)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.1524
_refine_ls_wR_factor_ref         0.1893
_reflns_number_gt                6552
_reflns_number_total             14471
_reflns_threshold_expression     >2sigma(I)
_cod_data_source_file            JSSC-2016-243-1.cif
_cod_data_source_block           xn_10_3
_cod_depositor_comments
;
The following automatic conversions were performed:

data item '_symmetry_cell_setting' value 'Tetragonal' was changed to
'tetragonal' in accordance with the built-in table derived from the
CIF Core dictionary named 'cif_core.dic' version 2.4.5 last updated
on 2014-11-21.

Automatic conversion script
Id: cif_fix_values 8369 2020-08-20 11:38:08Z andrius 
;
_cod_original_sg_symbol_H-M      P-42(1)c
_cod_database_code               1561331
loop_
_symmetry_equiv_pos_as_xyz
'x, y, z'
'-x, -y, z'
'y, -x, -z'
'-y, x, -z'
'-x+1/2, y+1/2, -z+1/2'
'x+1/2, -y+1/2, -z+1/2'
'-y+1/2, -x+1/2, z+1/2'
'y+1/2, x+1/2, z+1/2'
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_symmetry_multiplicity
_atom_site_calc_flag
_atom_site_refinement_flags
_atom_site_disorder_assembly
_atom_site_disorder_group
O1 O 0.2614(13) 0.2161(13) 0.5027(12) 0.032(9) Uani 1 1 d U . .
O2 O 0.2217(13) 0.2857(13) 0.4165(11) 0.027(8) Uani 1 1 d U . .
O3 O 0.3228(11) 0.3012(12) 0.2891(11) 0.018(8) Uani 1 1 d U . .
O5 O 0.3597(12) 0.2229(12) 0.5342(11) 0.022(8) Uani 1 1 d U . .
O6 O 0.4327(13) 0.2430(14) 0.2886(12) 0.035(10) Uani 1 1 d U . .
O7 O 0.4468(13) 0.1404(13) 0.3166(11) 0.025(8) Uani 1 1 d U . .
O8 O 0.3413(13) 0.1947(13) 0.3254(11) 0.027(7) Uani 1 1 d U . .
O10 O 0.3712(14) 0.1337(14) 0.4010(12) 0.033(7) Uani 1 1 d U . .
O12 O 0.3323(12) 0.2887(12) 0.4517(10) 0.017(6) Uani 1 1 d U . .
O13 O 0.1313(15) 0.2492(16) 0.3689(13) 0.050(10) Uani 1 1 d U . .
O14 O 0.5004(12) 0.2421(12) 0.3635(10) 0.015(7) Uani 1 1 d U . .
O15 O 0.5267(11) 0.2939(11) 0.4449(10) 0.016(7) Uani 1 1 d U . .
O16 O 0.4501(13) 0.2802(13) 0.5419(11) 0.030(9) Uani 1 1 d U . .
O17 O 0.4976(11) 0.3723(12) 0.6022(10) 0.014(7) Uani 1 1 d U . .
O18 O 0.4953(12) 0.3747(13) 0.5147(11) 0.023(8) Uani 1 1 d U . .
O22 O 0.4268(11) 0.2455(11) 0.4484(10) 0.014(6) Uani 1 1 d U . .
O23 O 0.2857(13) 0.3513(12) 0.3688(11) 0.025(8) Uani 1 1 d U . .
O24 O 0.2066(14) 0.3943(13) 0.4336(12) 0.036(9) Uani 1 1 d U . .
O25 O 0.3231(13) 0.4134(13) 0.2899(11) 0.028(8) Uani 1 1 d U . .
O26 O 0.4190(13) 0.3506(14) 0.2953(12) 0.032(9) Uani 1 1 d U . .
O27 O 0.5257(14) 0.3096(14) 0.2831(12) 0.041(10) Uani 1 1 d U . .
O28 O 0.5062(13) 0.1974(13) 0.4948(11) 0.026(9) Uani 1 1 d U . .
O30 O 0.4122(14) 0.3228(13) 0.6306(11) 0.030(9) Uani 1 1 d U . .
O31 O 0.3553(13) 0.3291(13) 0.5446(12) 0.033(9) Uani 1 1 d U . .
O32 O 0.1793(15) 0.1872(15) 0.4351(14) 0.049(10) Uani 1 1 d U . .
O33 O 0.1576(17) 0.0924(17) 0.2566(15) 0.063(12) Uani 1 1 d U . .
O34 O 0.2455(14) 0.2654(14) 0.2220(13) 0.040(9) Uani 1 1 d U . .
O35 O 0.3474(13) 0.2110(13) 0.2351(11) 0.025(8) Uani 1 1 d U . .
O36 O 0.4497(15) 0.1617(16) 0.2181(14) 0.049(11) Uani 1 1 d U . .
O37 O 0.3811(12) 0.4052(12) 0.3731(10) 0.017(8) Uani 1 1 d U . .
O38 O 0.5855(13) 0.2034(14) 0.4226(11) 0.031(8) Uani 1 1 d U . .
O39 O 0.4184(11) 0.3476(11) 0.4522(9) 0.012(6) Uani 1 1 d U . .
O40 O 0.4045(16) 0.0480(16) 0.3390(14) 0.058(12) Uani 1 1 d U . .
O41 O 0.3687(16) 0.1062(16) 0.2638(13) 0.056(12) Uani 1 1 d U . .
O42 O 0.4705(10) 0.4373(10) 0.4354(9) 0.006(6) Uani 1 1 d U . .
O43 O 0.2685(18) 0.0599(17) 0.2682(15) 0.070(14) Uani 1 1 d U . .
O44 O 0.2988(18) -0.0031(17) 0.3418(15) 0.067(13) Uani 1 1 d U . .
O45 O 0.2499(17) 0.1697(16) 0.2613(15) 0.058(12) Uani 1 1 d U . .
O46 O 0.2956(15) 0.1045(15) 0.3489(13) 0.045(8) Uani 1 1 d U . .
O47 O 0.3271(16) 0.0350(16) 0.4336(15) 0.059(12) Uani 1 1 d U . .
O48 O 0.2264(17) 0.0878(16) 0.4350(14) 0.062(12) Uani 1 1 d U . .
O49 O 0.1861(15) 0.1572(15) 0.3467(14) 0.052(11) Uani 1 1 d U . .
O50 O 0.204(2) 0.049(2) 0.3448(17) 0.093(16) Uani 1 1 d U . .
O51 O 0.4318(15) 0.0547(15) 0.4335(14) 0.049(11) Uani 1 1 d U . .
O52 O 0.5090(16) 0.0572(15) 0.3574(14) 0.050(10) Uani 1 1 d U . .
O53 O 0.3789(16) 0.0359(16) 0.5207(14) 0.055(10) Uani 1 1 d U . .
O54 O 0.4519(14) 0.1786(14) 0.5851(13) 0.041(9) Uani 1 1 d U . .
O55 O 0.4103(13) 0.1395(13) 0.4996(11) 0.023(8) Uani 1 1 d U . .
O56 O 0.4879(13) 0.1493(13) 0.4108(11) 0.027(8) Uani 1 1 d U . .
O57 O 0.2029(17) 0.1278(16) 0.5232(14) 0.059(11) Uani 1 1 d U . .
O58 O 0.2732(15) 0.2700(14) 0.5901(13) 0.044(10) Uani 1 1 d U . .
O59 O 0.2538(13) 0.3285(13) 0.5010(11) 0.027(9) Uani 1 1 d U . .
O60 O 0.2771(13) 0.1821(12) 0.4038(12) 0.028(7) Uani 1 1 d U . .
O61 O 0.2360(15) 0.2494(16) 0.3212(14) 0.053(11) Uani 1 1 d U . .
O62 O 0.3919(11) 0.2929(12) 0.3746(10) 0.016(6) Uani 1 1 d U . .
O63 O 0.4908(11) 0.3527(11) 0.3717(10) 0.012(7) Uani 1 1 d U . .
O78 O 0.3180(12) 0.4022(12) 0.4507(10) 0.019(8) Uani 1 1 d U . .
O79 O 0.3993(13) 0.4218(12) 0.5180(11) 0.023(8) Uani 1 1 d U . .
O80 O 0.3103(16) 0.1228(15) 0.4903(13) 0.049(11) Uani 1 1 d U . .
O81 O 0.2239(17) -0.0291(16) 0.4143(15) 0.065(8) Uani 1 1 d U . .
O82 O 0.3965(11) 0.4218(11) 0.6026(10) 0.010(7) Uani 1 1 d U . .
O180 O 0.3647(18) -0.0064(19) 0.2504(15) 0.075(15) Uani 1 1 d U . .
O1W O 0.320(4) 0.575(4) 0.811(3) 0.26(4) Uani 1 1 d U . .
O2W O 0.4916(15) 0.2651(16) 0.6797(13) 0.050(11) Uani 1 1 d U . .
O3W O 0.608(2) 0.063(2) 0.414(2) 0.103(18) Uani 1 1 d U . .
O5W O 0.5000 0.0000 0.544(5) 0.27(6) Uani 1 2 d SU . .
O6W O 0.271(5) 0.898(5) 0.743(4) 0.34(6) Uani 1 1 d U . .
O7W O 0.564(2) 0.098(2) 0.516(2) 0.12(2) Uani 1 1 d U . .
O8W O 0.1958(19) 0.3639(19) 0.2931(17) 0.085(15) Uani 1 1 d U . .
O9W O 0.093(9) 0.391(9) 0.321(8) 0.28(10) Uani 0.50 1 d PU . .
O10W O 0.147(2) 0.308(2) 0.547(2) 0.14(2) Uani 1 1 d U . .
O11W O 0.363(3) 0.210(3) 0.662(2) 0.15(3) Uani 1 1 d U . .
O14W O 0.305(3) 0.337(3) 0.673(2) 0.15(3) Uani 1 1 d U . .
O15W O 0.017(5) 0.232(5) 0.321(4) 0.30(5) Uani 1 1 d U . .
O17W O 0.318(3) 0.134(3) 0.613(2) 0.17(3) Uani 1 1 d U . .
O18W O 0.640(3) 0.088(3) 0.578(3) 0.17(3) Uani 1 1 d U . .
O20W O 0.976(10) 0.047(9) 0.258(9) 0.34(12) Uani 0.50 1 d PU . .
O22W O 0.559(5) 0.011(6) 0.782(5) 0.15(4) Uani 0.50 1 d PU . .
O23W O 0.091(4) 0.272(4) 0.477(4) 0.10(4) Uani 0.50 1 d PU . .
O24W O 0.471(4) 0.091(4) 0.666(3) 0.07(3) Uani 0.50 1 d PU . .
O26W O 0.068(4) 0.330(4) 0.193(4) 0.27(5) Uani 1 1 d U . .
O27W O 0.506(13) 0.003(17) 0.758(3) 0.14(4) Uani 0.50 1 d PU . .
P1 P 0.3215(6) 0.1577(6) 0.3709(5) 0.027(3) Uani 1 1 d U . .
P2 P 0.3929(4) 0.2925(4) 0.4303(4) 0.006(2) Uani 1 1 d U . .
Ta1 Ta 0.42782(8) 0.35703(8) 0.55816(7) 0.0157(5) Uani 1 1 d U . .
Ta2 Ta 0.51341(8) 0.37291(8) 0.44138(7) 0.0146(4) Uani 1 1 d U . .
Ta3 Ta 0.39033(8) 0.43590(8) 0.44294(7) 0.0155(4) Uani 1 1 d U . .
W1 W 0.43717(10) 0.20692(9) 0.52953(8) 0.0302(6) Uani 1 1 d U . .
W2 W 0.30188(9) 0.27451(9) 0.53239(9) 0.0321(6) Uani 1 1 d U . .
W3 W 0.26140(8) 0.35234(9) 0.43570(9) 0.0294(6) Uani 1 1 d U . .
W4 W 0.34904(9) 0.36406(9) 0.32623(8) 0.0261(5) Uani 1 1 d U . .
W5 W 0.47227(9) 0.30194(10) 0.32400(7) 0.0281(6) Uani 1 1 d U . .
W6 W 0.51853(9) 0.22016(8) 0.42953(8) 0.0230(5) Uani 1 1 d U . .
W7 W 0.37182(13) 0.08059(10) 0.47342(10) 0.0536(8) Uani 1 1 d U . .
W8 W 0.23575(11) 0.14871(11) 0.47652(10) 0.0526(8) Uani 1 1 d U . .
W9 W 0.19477(10) 0.22615(11) 0.37959(10) 0.0451(7) Uani 1 1 d U . .
W10 W 0.28285(10) 0.23900(10) 0.26855(9) 0.0373(7) Uani 1 1 d U . .
W11 W 0.40647(10) 0.17625(10) 0.26649(9) 0.0400(7) Uani 1 1 d U . .
W12 W 0.45270(11) 0.09394(9) 0.37342(10) 0.0424(7) Uani 1 1 d U . .
W13 W 0.25741(15) 0.02783(12) 0.39458(12) 0.0746(10) Uani 1 1 d U . .
W14 W 0.33998(13) 0.04153(11) 0.29327(11) 0.0602(9) Uani 1 1 d U . .
W15 W 0.21430(12) 0.10526(12) 0.29624(10) 0.0550(8) Uani 1 1 d U . .
O30W O 0.164(2) 0.450(2) 0.349(2) 0.12(2) Uani 1 1 d U . .
O31W O 0.916(3) 0.961(3) 0.192(2) 0.16(3) Uani 1 1 d U . .
O33W O 0.590(4) 0.045(4) 0.738(3) 0.21(4) Uani 1 1 d U . .
O34W O 0.182(5) 0.179(5) 0.628(5) 0.39(7) Uani 1 1 d U . .
O35W O 0.095(3) 0.092(3) 0.403(2) 0.14(2) Uani 1 1 d U . .
O40W O 0.424(6) 0.038(6) 0.634(5) 0.43(8) Uani 1 1 d U . .
O42W O 0.135(4) 0.945(4) 0.319(4) 0.27(5) Uani 1 1 d U . .
O41W O 0.023(6) 0.118(6) 0.315(5) 0.43(8) Uani 1 1 d U . .
O43W O 0.223(4) 0.345(4) 0.655(3) 0.23(4) Uani 1 1 d U . .
O44W O 0.066(8) 0.051(8) 0.566(8) 0.29(10) Uani 0.50 1 d PU . .
O45W O 0.342(11) 0.370(11) 0.685(9) 0.13(3) Uani 0.25 1 d PU . .
O48W O 0.960(4) 0.277(4) 0.394(3) 0.25(4) Uani 1 1 d U . .
loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
O O 0.0106 0.0060 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
P P 0.1023 0.0942 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Ta Ta -0.7052 6.5227 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
W W -0.8490 6.8722 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
W8 O1 W2 166.9(19) . .
W9 O2 W3 162.2(18) . .
W10 O3 W4 163.2(17) . .
W2 O5 W1 149.5(17) . .
W11 O6 W5 165(2) . .
W11 O7 W12 152.9(18) . .
P1 O8 W11 129.5(18) . .
P1 O8 W10 125.6(18) . .
W11 O8 W10 92.7(11) . .
P1 O10 W12 129.8(19) . .
P1 O10 W7 130(2) . .
W12 O10 W7 92.1(11) . .
P2 O12 W3 125.0(16) . .
P2 O12 W2 130.2(16) . .
W3 O12 W2 92.2(10) . .
W5 O14 W6 143.8(16) . .
W6 O15 Ta2 157.7(16) . .
W1 O16 Ta1 154.2(19) . .
Ta3 O17 Ta1 109.1(12) 4_656 .
Ta3 O18 Ta2 111.9(14) 4_656 .
Ta3 O18 Ta1 111.2(13) 4_656 .
Ta2 O18 Ta1 136.5(16) . .
P2 O22 W6 130.3(16) . .
P2 O22 W1 131.1(16) . .
W6 O22 W1 90.0(9) . .
W3 O23 W4 143.7(17) . .
W4 O26 W5 121.5(16) . .
W6 O28 W1 124.3(17) . .
W2 O31 Ta1 155.9(19) . .
W9 O32 W8 124.5(19) . .
W11 O35 W10 124.4(16) . .
W4 O37 Ta3 154.9(17) . .
P2 O39 Ta3 129.6(15) . .
P2 O39 Ta2 123.0(15) . .
Ta3 O39 Ta2 91.9(9) . .
W12 O40 W14 148(2) . .
W14 O41 W11 152(2) . .
Ta2 O42 Ta3 121.8(13) . .
W15 O43 W14 129(2) . .
W14 O44 W13 124(2) . .
W10 O45 W15 146(2) . .
P1 O46 W14 126(2) . .
P1 O46 W13 127(2) . .
W14 O46 W13 90.3(12) . .
P1 O46 W15 123(2) . .
W14 O46 W15 89.9(12) . .
W13 O46 W15 89.8(12) . .
W7 O47 W13 147(2) . .
W8 O48 W13 151(2) . .
W9 O49 W15 147(2) . .
W15 O50 W13 126(3) . .
W7 O51 W12 120.5(19) . .
W7 O55 W1 169(2) . .
W12 O56 W6 160.8(18) . .
W3 O59 W2 124.2(17) . .
P1 O60 W9 127.8(19) . .
P1 O60 W8 131.4(18) . .
W9 O60 W8 91.6(11) . .
W10 O61 W9 155(2) . .
P2 O62 W5 124.1(16) . .
P2 O62 W4 123.9(16) . .
W5 O62 W4 88.4(9) . .
W5 O63 Ta2 151.9(16) . .
W3 O78 Ta3 155.2(16) . .
Ta2 O79 Ta1 114.6(14) 3_566 .
Ta2 O79 Ta3 111.9(14) 3_566 .
Ta1 O79 Ta3 133.5(15) . .
W7 O80 W8 150(2) . .
Ta2 O82 Ta1 109.7(12) 3_566 .
O27W O22W O27W 6(10) . 2_655
O27W O27W O22W 148(10) 2_655 .
O27W O27W O22W 26(10) 2_655 2_655
O22W O27W O22W 132(10) . 2_655
O60 P1 O46 105.2(19) . .
O60 P1 O10 112.5(19) . .
O46 P1 O10 101.6(19) . .
O60 P1 O8 116.7(18) . .
O46 P1 O8 106.9(19) . .
O10 P1 O8 112.4(19) . .
O22 P2 O62 110.1(17) . .
O22 P2 O12 110.3(16) . .
O62 P2 O12 110.6(16) . .
O22 P2 O39 107.7(16) . .
O62 P2 O39 112.0(16) . .
O12 P2 O39 105.9(15) . .
O31 Ta1 O16 82.9(14) . .
O31 Ta1 O79 81.9(13) . .
O16 Ta1 O79 134.2(12) . .
O31 Ta1 O18 133.7(13) . .
O16 Ta1 O18 81.5(12) . .
O79 Ta1 O18 78.6(12) . .
O31 Ta1 O17 155.1(12) . .
O16 Ta1 O17 94.1(12) . .
O79 Ta1 O17 116.2(12) . .
O18 Ta1 O17 69.5(11) . .
O31 Ta1 O82 92.4(13) . .
O16 Ta1 O82 156.5(11) . .
O79 Ta1 O82 67.1(11) . .
O18 Ta1 O82 117.1(11) . .
O17 Ta1 O82 80.5(11) . .
O31 Ta1 O30 83.0(13) . .
O16 Ta1 O30 83.7(12) . .
O79 Ta1 O30 136.3(12) . .
O18 Ta1 O30 137.5(12) . .
O17 Ta1 O30 72.1(11) . .
O82 Ta1 O30 72.9(11) . .
O42 Ta2 O15 155.8(11) . .
O42 Ta2 O79 102.4(12) . 4_656
O15 Ta2 O79 99.0(12) . 4_656
O42 Ta2 O63 88.3(11) . .
O15 Ta2 O63 81.5(11) . .
O79 Ta2 O63 142.6(11) 4_656 .
O42 Ta2 O18 87.0(12) . .
O15 Ta2 O18 90.5(12) . .
O79 Ta2 O18 68.2(12) 4_656 .
O63 Ta2 O18 148.9(11) . .
O42 Ta2 O82 98.2(11) . 4_656
O15 Ta2 O82 100.1(11) . 4_656
O79 Ta2 O82 68.6(11) 4_656 4_656
O63 Ta2 O82 74.5(11) . 4_656
O18 Ta2 O82 136.6(11) . 4_656
O42 Ta2 O39 72.1(10) . .
O15 Ta2 O39 84.3(11) . .
O79 Ta2 O39 139.4(10) 4_656 .
O63 Ta2 O39 78.1(10) . .
O18 Ta2 O39 71.3(10) . .
O82 Ta2 O39 151.1(10) 4_656 .
O42 Ta2 Ta3 29.7(8) . .
O15 Ta2 Ta3 126.5(8) . .
O79 Ta2 Ta3 122.7(9) 4_656 .
O63 Ta2 Ta3 83.2(8) . .
O18 Ta2 Ta3 77.6(9) . .
O82 Ta2 Ta3 124.2(8) 4_656 .
O39 Ta2 Ta3 42.4(7) . .
O42 Ta3 O78 156.1(11) . .
O42 Ta3 O18 103.2(11) . 3_566
O78 Ta3 O18 96.6(12) . 3_566
O42 Ta3 O37 91.0(11) . .
O78 Ta3 O37 81.3(12) . .
O18 Ta3 O37 142.2(11) 3_566 .
O42 Ta3 O79 90.1(11) . .
O78 Ta3 O79 85.4(12) . .
O18 Ta3 O79 66.8(12) 3_566 .
O37 Ta3 O79 149.2(11) . .
O42 Ta3 O17 97.8(11) . 3_566
O78 Ta3 O17 101.5(12) . 3_566
O18 Ta3 O17 70.2(10) 3_566 3_566
O37 Ta3 O17 73.3(11) . 3_566
O79 Ta3 O17 136.9(11) . 3_566
O42 Ta3 O39 74.2(10) . .
O78 Ta3 O39 82.1(10) . .
O18 Ta3 O39 139.5(11) 3_566 .
O37 Ta3 O39 77.9(10) . .
O79 Ta3 O39 72.8(11) . .
O17 Ta3 O39 150.0(10) 3_566 .
O42 Ta3 Ta2 28.5(7) . .
O78 Ta3 Ta2 127.7(8) . .
O18 Ta3 Ta2 122.7(9) 3_566 .
O37 Ta3 Ta2 85.4(8) . .
O79 Ta3 Ta2 81.0(9) . .
O17 Ta3 Ta2 122.4(8) 3_566 .
O39 Ta3 Ta2 45.7(7) . .
O54 W1 O16 101.2(15) . .
O54 W1 O55 95.8(14) . .
O16 W1 O55 162.0(13) . .
O54 W1 O5 103.2(15) . .
O16 W1 O5 87.7(13) . .
O55 W1 O5 82.5(13) . .
O54 W1 O28 101.8(15) . .
O16 W1 O28 93.2(13) . .
O55 W1 O28 89.2(13) . .
O5 W1 O28 154.4(13) . .
O54 W1 O22 173.7(14) . .
O16 W1 O22 79.0(11) . .
O55 W1 O22 84.8(11) . .
O5 W1 O22 83.1(11) . .
O28 W1 O22 72.0(11) . .
O58 W2 O31 99.4(15) . .
O58 W2 O5 103.6(15) . .
O31 W2 O5 87.1(13) . .
O58 W2 O1 97.5(15) . .
O31 W2 O1 162.5(14) . .
O5 W2 O1 84.3(13) . .
O58 W2 O59 101.5(15) . .
O31 W2 O59 91.0(13) . .
O5 W2 O59 154.8(13) . .
O1 W2 O59 90.4(13) . .
O58 W2 O12 172.9(14) . .
O31 W2 O12 81.0(12) . .
O5 W2 O12 83.5(11) . .
O1 W2 O12 82.8(12) . .
O59 W2 O12 71.4(11) . .
O24 W3 O78 101.3(14) . .
O24 W3 O59 98.1(15) . .
O78 W3 O59 93.8(13) . .
O24 W3 O23 102.8(15) . .
O78 W3 O23 89.3(12) . .
O59 W3 O23 157.9(13) . .
O24 W3 O2 95.8(14) . .
O78 W3 O2 162.5(12) . .
O59 W3 O2 87.1(13) . .
O23 W3 O2 83.5(12) . .
O24 W3 O12 170.2(13) . .
O78 W3 O12 81.2(11) . .
O59 W3 O12 72.3(12) . .
O23 W3 O12 86.6(12) . .
O2 W3 O12 82.4(11) . .
O25 W4 O37 100.6(14) . .
O25 W4 O26 101.3(14) . .
O37 W4 O26 91.2(14) . .
O25 W4 O3 97.6(14) . .
O37 W4 O3 161.8(13) . .
O26 W4 O3 85.9(13) . .
O25 W4 O23 99.6(14) . .
O37 W4 O23 90.6(13) . .
O26 W4 O23 158.3(13) . .
O3 W4 O23 85.6(13) . .
O25 W4 O62 176.0(13) . .
O37 W4 O62 79.9(11) . .
O26 W4 O62 74.7(11) . .
O3 W4 O62 82.0(11) . .
O23 W4 O62 84.4(11) . .
O27 W5 O63 101.4(14) . .
O27 W5 O14 100.0(14) . .
O63 W5 O14 91.5(12) . .
O27 W5 O26 100.3(15) . .
O63 W5 O26 92.2(13) . .
O14 W5 O26 158.2(13) . .
O27 W5 O6 97.5(15) . .
O63 W5 O6 161.0(13) . .
O14 W5 O6 84.1(13) . .
O26 W5 O6 85.4(14) . .
O27 W5 O62 174.5(13) . .
O63 W5 O62 81.8(11) . .
O14 W5 O62 84.3(11) . .
O26 W5 O62 75.0(12) . .
O6 W5 O62 79.4(11) . .
O38 W6 O15 99.0(14) . .
O38 W6 O28 100.8(14) . .
O15 W6 O28 95.1(13) . .
O38 W6 O14 100.6(14) . .
O15 W6 O14 88.1(12) . .
O28 W6 O14 157.6(13) . .
O38 W6 O56 97.2(15) . .
O15 W6 O56 163.3(13) . .
O28 W6 O56 85.7(13) . .
O14 W6 O56 85.0(12) . .
O38 W6 O22 173.7(13) . .
O15 W6 O22 78.5(11) . .
O28 W6 O22 73.8(12) . .
O14 W6 O22 85.2(11) . .
O56 W6 O22 85.8(12) . .
O53 W7 O80 104.3(17) . .
O53 W7 O55 98.8(15) . .
O80 W7 O55 83.4(15) . .
O53 W7 O47 96.8(18) . .
O80 W7 O47 90.1(16) . .
O55 W7 O47 164.2(15) . .
O53 W7 O51 98.1(18) . .
O80 W7 O51 157.5(16) . .
O55 W7 O51 95.0(14) . .
O47 W7 O51 85.5(16) . .
O53 W7 O10 171.1(15) . .
O80 W7 O10 84.2(14) . .
O55 W7 O10 84.4(12) . .
O47 W7 O10 80.7(14) . .
O51 W7 O10 73.3(14) . .
O57 W8 O48 99.7(18) . .
O57 W8 O1 98.2(17) . .
O48 W8 O1 161.8(16) . .
O57 W8 O80 102.2(17) . .
O48 W8 O80 88.5(16) . .
O1 W8 O80 84.3(15) . .
O57 W8 O32 104.7(17) . .
O48 W8 O32 86.9(16) . .
O1 W8 O32 91.9(14) . .
O80 W8 O32 153.1(15) . .
O57 W8 O60 174.9(16) . .
O48 W8 O60 79.5(14) . .
O1 W8 O60 83.0(12) . .
O80 W8 O60 82.9(13) . .
O32 W8 O60 70.2(13) . .
O13 W9 O32 97.3(17) . .
O13 W9 O2 98.9(16) . .
O32 W9 O2 91.7(15) . .
O13 W9 O49 96.4(17) . .
O32 W9 O49 84.8(16) . .
O2 W9 O49 164.6(15) . .
O13 W9 O61 103.6(16) . .
O32 W9 O61 157.9(16) . .
O2 W9 O61 91.8(15) . .
O49 W9 O61 86.0(16) . .
O13 W9 O60 170.0(15) . .
O32 W9 O60 73.1(14) . .
O2 W9 O60 84.6(12) . .
O49 W9 O60 80.0(14) . .
O61 W9 O60 85.6(13) . .
O34 W10 O61 101.5(16) . .
O34 W10 O45 91.9(17) . .
O61 W10 O45 86.7(17) . .
O34 W10 O3 101.2(15) . .
O61 W10 O3 88.7(14) . .
O45 W10 O3 166.7(16) . .
O34 W10 O35 102.6(15) . .
O61 W10 O35 155.7(14) . .
O45 W10 O35 88.9(15) . .
O3 W10 O35 90.3(12) . .
O34 W10 O8 172.1(14) . .
O61 W10 O8 85.7(14) . .
O45 W10 O8 85.2(15) . .
O3 W10 O8 82.1(11) . .
O35 W10 O8 70.1(12) . .
O36 W11 O6 102.6(16) . .
O36 W11 O35 102.2(16) . .
O6 W11 O35 91.0(14) . .
O36 W11 O7 98.1(16) . .
O6 W11 O7 89.5(14) . .
O35 W11 O7 159.0(13) . .
O36 W11 O41 94.6(17) . .
O6 W11 O41 161.9(15) . .
O35 W11 O41 90.8(14) . .
O7 W11 O41 82.4(15) . .
O36 W11 O8 174.0(15) . .
O6 W11 O8 80.8(13) . .
O35 W11 O8 72.6(12) . .
O7 W11 O8 86.8(12) . .
O41 W11 O8 82.6(14) . .
O52 W12 O40 93.6(18) . .
O52 W12 O56 98.5(16) . .
O40 W12 O56 167.9(16) . .
O52 W12 O7 99.4(15) . .
O40 W12 O7 84.3(15) . .
O56 W12 O7 92.8(13) . .
O52 W12 O51 99.7(16) . .
O40 W12 O51 88.0(16) . .
O56 W12 O51 90.8(14) . .
O7 W12 O51 159.8(14) . .
O52 W12 O10 172.2(15) . .
O40 W12 O10 82.9(15) . .
O56 W12 O10 85.2(12) . .
O7 W12 O10 87.2(12) . .
O51 W12 O10 73.3(13) . .
O81 W13 O44 99.8(19) . .
O81 W13 O50 97(2) . .
O44 W13 O50 85.9(19) . .
O81 W13 O48 104.1(18) . .
O44 W13 O48 155.7(17) . .
O50 W13 O48 86.7(18) . .
O81 W13 O47 108.0(18) . .
O44 W13 O47 89.3(17) . .
O50 W13 O47 155.4(19) . .
O48 W13 O47 87.9(16) . .
O81 W13 O46 167.2(16) . .
O44 W13 O46 73.5(16) . .
O50 W13 O46 72.4(17) . .
O48 W13 O46 82.2(14) . .
O47 W13 O46 83.1(14) . .
O180 W14 O41 98.2(18) . .
O180 W14 O43 103.2(19) . .
O41 W14 O43 89.4(17) . .
O180 W14 O44 104.6(19) . .
O41 W14 O44 157.1(17) . .
O43 W14 O44 84.6(18) . .
O180 W14 O40 101.3(19) . .
O41 W14 O40 84.8(16) . .
O43 W14 O40 155.3(17) . .
O44 W14 O40 91.4(17) . .
O180 W14 O46 173.4(17) . .
O41 W14 O46 84.5(14) . .
O43 W14 O46 70.7(15) . .
O44 W14 O46 72.7(15) . .
O40 W14 O46 84.8(14) . .
O33 W15 O43 101.2(18) . .
O33 W15 O50 101(2) . .
O43 W15 O50 87.0(19) . .
O33 W15 O49 105.3(17) . .
O43 W15 O49 153.5(16) . .
O50 W15 O49 86.4(18) . .
O33 W15 O45 100.5(18) . .
O43 W15 O45 87.9(17) . .
O50 W15 O45 158.4(19) . .
O49 W15 O45 88.9(16) . .
O33 W15 O46 169.2(16) . .
O43 W15 O46 70.5(15) . .
O50 W15 O46 72.2(17) . .
O49 W15 O46 83.0(13) . .
O45 W15 O46 86.3(14) . .
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
O1 W8 1.88(3) .
O1 W2 1.90(3) .
O2 W9 1.87(3) .
O2 W3 1.95(3) .
O3 W10 1.87(3) .
O3 W4 1.93(3) .
O5 W2 1.88(3) .
O5 W1 1.92(3) .
O6 W11 1.83(3) .
O6 W5 1.97(3) .
O7 W11 1.88(3) .
O7 W12 1.91(3) .
O8 P1 1.59(3) .
O8 W11 2.29(3) .
O8 W10 2.35(3) .
O10 P1 1.56(3) .
O10 W12 2.32(3) .
O10 W7 2.34(3) .
O12 P2 1.58(3) .
O12 W3 2.34(3) .
O12 W2 2.33(3) .
O13 W9 1.66(4) .
O14 W5 1.92(3) .
O14 W6 1.92(3) .
O15 W6 1.84(3) .
O15 Ta2 1.94(3) .
O16 W1 1.83(3) .
O16 Ta1 1.98(3) .
O17 Ta3 2.07(3) 4_656
O17 Ta1 2.10(3) .
O18 Ta3 2.06(3) 4_656
O18 Ta2 2.03(3) .
O18 Ta1 2.06(3) .
O22 P2 1.49(3) .
O22 W6 2.36(3) .
O22 W1 2.40(3) .
O23 W3 1.90(3) .
O23 W4 1.94(3) .
O24 W3 1.67(3) .
O25 W4 1.67(3) .
O26 W4 1.92(3) .
O26 W5 1.91(3) .
O27 W5 1.71(3) .
O28 W6 1.87(3) .
O28 W1 1.93(3) .
O30 Ta1 2.16(3) .
O31 W2 1.88(3) .
O31 Ta1 1.91(3) .
O32 W9 1.81(4) .
O32 W8 2.00(4) .
O33 W15 1.77(4) .
O34 W10 1.68(3) .
O35 W11 1.86(3) .
O35 W10 1.93(3) .
O36 W11 1.71(4) .
O37 W4 1.79(3) .
O37 Ta3 2.04(3) .
O38 W6 1.68(3) .
O39 P2 1.58(3) .
O39 Ta3 2.26(3) .
O39 Ta2 2.40(3) .
O40 W12 1.86(4) .
O40 W14 2.00(4) .
O41 W14 1.89(4) .
O41 W11 1.92(4) .
O42 Ta2 1.88(2) .
O42 Ta3 1.95(2) .
O43 W15 1.87(4) .
O43 W14 1.91(4) .
O44 W14 1.97(4) .
O44 W13 1.90(4) .
O45 W10 1.87(4) .
O45 W15 2.02(4) .
O46 P1 1.55(4) .
O46 W14 2.40(4) .
O46 W13 2.41(4) .
O46 W15 2.43(4) .
O47 W7 1.88(4) .
O47 W13 2.00(4) .
O48 W8 1.87(4) .
O48 W13 1.97(4) .
O49 W9 1.90(4) .
O49 W15 1.98(4) .
O50 W15 1.91(5) .
O50 W13 1.93(5) .
O51 W7 1.91(4) .
O51 W12 1.95(4) .
O52 W12 1.68(4) .
O53 W7 1.68(4) .
O54 W1 1.69(4) .
O55 W7 1.84(3) .
O55 W1 1.93(3) .
O56 W12 1.88(3) .
O56 W6 1.93(3) .
O57 W8 1.58(4) .
O58 W2 1.71(3) .
O59 W3 1.87(3) .
O59 W2 1.94(3) .
O60 P1 1.51(3) .
O60 W9 2.35(3) .
O60 W8 2.35(3) .
O61 W10 1.84(4) .
O61 W9 1.95(4) .
O62 P2 1.51(3) .
O62 W5 2.39(3) .
O62 W4 2.40(3) .
O63 W5 1.84(3) .
O63 Ta2 2.02(3) .
O78 W3 1.87(3) .
O78 Ta3 1.94(3) .
O79 Ta2 2.02(3) 3_566
O79 Ta1 2.03(3) .
O79 Ta3 2.07(3) .
O80 W7 1.86(4) .
O80 W8 1.94(4) .
O81 W13 1.68(4) .
O82 Ta2 2.05(3) 3_566
O82 Ta1 2.12(3) .
O180 W14 1.75(4) .
O14W O45W 1.2(3) .
O22W O27W 1.4(3) .
O22W O27W 1.7(3) 2_655
O27W O27W 0.3(6) 2_655
O27W O22W 1.7(3) 2_655
Ta2 O79 2.02(3) 4_656
Ta2 O82 2.05(3) 4_656
Ta2 Ta3 3.344(3) .
Ta3 O18 2.06(3) 3_566
Ta3 O17 2.07(3) 3_566
